advertisement

Phase-reversed structures in superlattice of nonlinear materials D. A. Antonosyan1, 2, ∗ and G. Yu. Kryuchkyan1, 2, † arXiv:1109.2751v1 [quant-ph] 13 Sep 2011 1 Yerevan State University, Alex Manoogian 1, 0025, Yerevan, Armenia 2 Institute for Physical Researches, National Academy of Sciences, Ashtarak-2, 0203, Ashtarak, Armenia We present detailed description of so-called phase-reversed structures that are characterized by two grating wave vectors allowing simultaneously phase-match two parametric three-wave processes. The novelty is that the structure is realized as a definite assembly of nonlinear segments leading to detailed description of cascaded three-photon processes with the parameters of realistic structured nonlinear materials of finite length. We apply these results for analysis of the quasi-phase-matching in production of both photon triplet and four-photon states in cascaded down-conversion. The received results are matched with the experimental data. Keywords: Multi-photon processes, quasi-phase-matching, phase-reversed superlattice, down-conversion. I. INTRODUCTION Cascading processes in optical materials that involve several different second-order nonlinear interactions provide an efficient way to lower the critical power of optical parametric devices. The concept of multistep cascading brings new ideas into this field, leading to the possibility of an enhanced nonlinearity-induced phase shift, the simultaneous generation of higher-order harmonics, multicolor parametric interaction, difference-frequency generation, (see, [1] and references therein). Multistep parametric interactions and multistep cascading are characterized by at least two different nearly phase-matching or quasiphase-matching (QPM) parameters. QPM is an important technique in nonlinear optics and is widespread used for various applications [1, 2]. The width of the phasematching curve depends on the type of the crystal, its length, and the phase-matching method. QPM not only makes efficient frequency conversion possible, but also enables diverse applications such as beam and pulse shaping, multi-harmonic generation, high harmonic generation and all-optical processing. Recently, it has been demonstrated that the quantum-computational gates, multimode quantum interference of photons and preparation of multi-photon entangled states also can be realized d + - ... - - ... + + ... Lph FIG. 1: Scheme of periodically poled nonlinear crystal (PPNC) which involves nonlinear domains of length l with χ+ > 0 and χ− < 0 with phase-reversal grating (with period Λph ) upon a uniform QPM grating (with period d). ∗ [email protected] † [email protected] in QPM structures [3–6]. One of the non-uniform QPM structures is so-called phase-reversed structures [7], which has been studied both theoretically and experimentally and have been employed for the wavelength conversion, and for the cascaded single-crystal third harmonic generation process [8, 9]. Several proposals for increasing the phasematching region have also been suggested, including the use of the phase-reversed QPM structures. These structures are based on the use of a phase-reversed sequence of many equivalent uniform short QPM domains, particularly, periodically poled domains, in which neighboring nonlinear segments have the opposite signs of the second-order susceptibility. The phase-reversed structures arranged in such a way that at the place of the joint two ends of the domains segments have the same sign of the χ(2) coefficient (see Fig. 1). On the whole, this structure is characterized by two grating wave vectors allowing phase-match two processes. In the standard approach, the one-dimensional χ(2) (z) function leading to the phase-reversed QPM structure can be described by the infinite Fourier expansion on two periods. Such phenomenological approach qualitatively explains the simultaneous QPM of two parametric nonlinear processes, however, has not included the parameters of realistic structured nonlinear materials. These dates often should be taken into to consideration if we are interest in more detailed description of cascaded parametric processes. In this paper, we present more detailed description of phase-reversed structures in another way as the definite assembly of nonlinear segments. Then, we arrange this structure for two cascaded parametric devices proposed for generation of three-photon and four-photon states. In this way, we consider cascaded collinear parametric processes in one dimensional media. The paper is arranged as follows. In Sec. II we consider an effective nonlinear coefficient G(∆k) of three-wave interaction in one-dimensional phase-reversed media. This quantity is defined as the Fourier transform of the second order susceptibility χ(2) (z) in term of wave vectors mismatch ∆k of three-wave interaction caused by dispersion in an optical material. In Sec.III we briefly consider application of 2 these results for obtaining QPM in generation of multiphotonic states. II. PHASE-REVERSED STRUCTURES OF FINITE LENGHT We start with consideration of effective coupling constant G(∆k) that usually describe three-wave interaction in second-order nonlinear media with the susceptibility χ(2) (z) in the following form G(∆k) = Z L χ(2) (z)ei∆k(z) dz, (1) where ∆k is the phase-matching parameter and L is a length of medium. In the phenomenological approach the χ(2) (z) function leading to the phase-reversed QPM structure can be described by the following Fourier expansion χ(2) (z) = χ0 ∞ X gn eiGn z n=−∞ ∞ X gm eiFm z , (2) m=−∞ that is the product of two periodic functions. Here: g0 = 0, gn6=0 = 2/πn, gm6=0 = 2/πm and Gn = 2π d n, Fm = Λ2π m. In this case the effective interaction conph stant reads as 0 G(∆k) = χ0 L ∞ X ∞ X gn gm e −i L 2 (∆k−Gn −Fm ) n=−∞ m=−∞ Considering the phase-reversed QPM structure as the definite assembly of nonlinear segments we turn to the general formula obtained for the effective coupling constant in multilayered media [10] G (∆k) = X l m χm e lm −i(ϕm + ∆km ) 2 sinc m ϕm = m−1 X ln ∆kn , (4) n where ∆kn = k0n − k1n − k2n is the phase-matching function of three photon process in the each n-th domain, YM,N (∆k) = sinc l∆k 2 YM,N (∆k) = sinc l∆k 2 ω (5) We assume that phase-matching parameters are the same for all layers ∆kn ≡ ∆k, as well as χ+ = |χ− | ≡ χ0 . We introduce the QPM function YM,N (∆k) which is the product of the standard phase-matching spectral function for a single segment, i.e. sinc l∆k , and the 2 assemble function l 1 sin [ N2 l (∆k − G)] sin [ MN 2 (∆k − F )] . M N sin [ 2l (∆k − G)] sin [ N2 l (∆k − F )] Here: N -is the number of domains in each block, M -is the number of blocks, α(∆k) = N2l [(∆k − G) + (M − 1)(∆k − F )], l-is the length of each domain, G = 2π/d, F = 2π/Λph , d = 2l, Λph = 2N l, L = M N l. It is easy to (3) kjn (z, ω) = cj nn (z, ωj ), nn (ω) is the refractive index of the medium at the given frequency. In the result, the effective nonlinear coefficient G(∆k) for the scheme depicted in the Fig.1 can be calculated in the following form G (∆k) = Lχ0 e−iα(∆k) YM,N (∆k). ∆km lm , 2 ϕ1 = 0, L (∆k − Gn − Fm ) . sinc 2 (6) check that the function YM,N (∆k) has an alternative representation, as the product of expansions on the number of domains and blocks N M 1 iϕ X −il(n∆k−Gn ) X −iN l(m∆k−Fm ) e e e , MN n=1 m=1 (7) 3 where ϕ = 2l (∆k − G). As we see, the above expressions (5), (7) derived on the base of the method of superlatices elaborated on the multilayered media differs from the formula (3), which is obtained in the standard, phenomenological approach. In contrast to the expression (3), the results (6),(7) depend on the number of the domains and blocks and also describe the case of small numbers of the segments. It is remarkable, that in this case the QPM function displays specific interference effects. Nevertheless, as shows our analysis some consequences of both (3) and (5) results, for N ≫ 1, M ≫ 1, coincide qualitatively. Note, that single-phase-matched process of threephoton interaction in multilayered media is also described by an assembly function. For PPLN structure (see, one of the block in Fig.1 containing N layers) the phasematching function is calculated as YN (∆k) = sinc l∆k 2 1 sin [ N2l (∆k − G)] , N sin [ 2l (∆k − G)] 0.4 Y 8,22 x 0.2 1.5 0.4 1.6 1.7 -0.2 0.2 -6 -4 2 -2 x 4 -0.2 FIG. 2: Plot of the function YM,N (x) for even numbers of both domains and blocks; N = 22 and M = 8. The inset shows the twin narrow peaks of opposite amplitudes. 0.4 (8) where ∆k is the wave vectors mismatch of three-wave interaction. This function exhibits a structure of single narrow peaks as discussed in [11]. The obtained QPM function YM,N (∆k) allows simultaneously phase-match two parametric processes which is achieved by using two grating vectors. In order to illustrate the possibility of the double phase-matching in such superlattice structure we present a detailed analysis of the function YM,N (x) in dependence on the parameter x = l∆k 2 in the graphical form (see, Figs. 2, 3). The assembly function exhibits the structure of peaks that are separated by π. Unlike to the assembly function for single-phase-matched process, YN (∆k) function has more complex structure, particularly, each group of the extremes consists of thin structure of twin-narrow peaks, separated by oscillating low maxima. The sinc l∆k 2 multiplier causes decreasing the amplitude of the consecutive peaks. The behavior of YM,N (x) function is different for even and odd values of M . As depicted in Fig. 2 for even values of M the twin peaks have the opposite signs, while for odd values of M the both narrow peaks have the same sign (see Fig. 3). The existence of twin peaks and oscillation between them are the main peculiarities of this structure. These twin narrow peaks can be chosen to phase-match two parametric processes involved into the multistep-cascading. Here we represent YM,N (∆k) function for the small number of domains to exhibit direct correlation between number of domains and the width of phase-matching function (see, Fig. 4). It is easy to notice that with the decrease of number of domains and blocks the narrow peaks in the pase-matching function becomes wider, as well as the number of oscillation between twin peaks decreases. Besides this, the positions of the maxima of the phasematching function becomes slightly shifted, although the periodicity of the YM,N (x) function is remained the same. Y 9,22 x 0.4 0.3 0.2 0.1 1.5 0.2 -6 -4 -2 1.6 1.7 -0.1 2 4 x -0.2 FIG. 3: Plot of the function YM,N (x) for even numbers of N = 22 and odd numbers M = 9. The inset shows the twin narrow peaks of the same amplitudes. III. APPLICATIONS: QPM FOR PRODUCTION OF MULIPHOTON STATES In this section, we apply the above results analyzing the QPM in generation of both photon triplet and fourphoton states in cascaded down-conversion. Recently, production of joint multiphoton states, particularly, photon triplet have attracted a great interest in probing the foundations of quantum theory and for various applications in quantum information technologies (see, [12–15] and the references therein). Depending on the configuration of the experiment and the designs of the crystal, the multiphoton states can be entangled in any number of variables: time, frequency, direction of propagation, and polarization. Studies carried out with miltiphoton state beams range from the examination of quantum paradoxes, to applications in optical measurements, spectroscopy, imaging, and quantum information (see, [13, 16] and references there). In this way, the direct generation of photon triplets using cascaded photon-pairs has been 4 where x1 = l∆k1 /2, x2 = l∆k2 /2. In general, the ampli′ tude of three-photons at the frequencies ω1 , ω1 , ω1” generated in cascaded down-conversion has been calculated in [15]. This quantity is proportional to the factor E0 ζξ. For the case of phase-reverse structure we can calculate three-photon amplitude in the following form 0.4 Y 2,6 x 0.2 0.4 1.0 1.5 2.0 -0.2 0.2 -6 -4 -2 -0.2 2 4 x ′ Φ(ω1 , ω1 , ω1” ) = f (ω1 , ω2 )h(∆k1 , ∆k2 ), (11) h(∆k1 , ∆k2 ) = (M N )2 YM,N (k1 )YM,N (k2 ) (12) where FIG. 4: Plot of the function YM,N (x) for the small numbers of domains and blocks, namely N = 6 and M = 2. The insert shows the broadening of the peaks. demonstrated in periodically poled lithium niobate crystals [14]. Most recently, joint quantum states of threephotons with arbitrary spectral characteristics have been studied on the base of optical superlattises [15]. In continuous of this paper, we analyze the cascaded generation of photon triplets in phase-reversed superlattice of χ(2) materials. We consider collinear, one-dimensional configurations focusing on consideration of cascaded parametric downconversion (PDC), which generates three-photon states in the presence of an optical cavity. In the scheme considered the pump field at the frequency ω0 converts to the subharmonics at the central frequencies ω1 = ω30 and ω2 = 2ω3 0 throughout two cascaded processes: ω0 → ω1 + ω2 and ω2 → ω1 + ω1 . Below we consider the amplitude of three-photon generation through the cascaded processes assuming the frequencies ω1 and ω2 as variable quantities distributed around the central values ω30 and 2ω0 3 , respectively. These processes are characterized by the wave-vector mismatches: ∆k1 = k(ω0 )−k(ω1 )−k(ω2 ) ′ and ∆k2 = k(ω2 ) − k(ω1 ) − k(ω1” ). The model Hamiltonian for the system, in the rotating-wave approximation, is given by ∗ iω0 t Hint = i~ E0 e−iω0 t a+ a0 + 0 − E0 e +2 i~ζ a0 a+ b+ − a+ b − a2 b + . 0 ab + i~ξ a (9) Here, ζ and ξ are the nonlinear coupling constants that are the Fourier transformations of the second-order nonlinear susceptibility χ(2) (z) ( see, Eq.(1)). The cavity modes are described by discreet creation and annihilation operators a+ , b+ and a, b as E0 describes the amplitude of the driving fields. For the case of the phasereversed superlattice structure the constants of the processes ω0 → ω1 + ω2 and ω2 → ω1 + ω1 are calculated as ζ ∼ Le−iα(∆k1 ) YM,N (x1 ), ξ ∼ Le−iα(∆k2 ) YM,N (x2 ), (10) is the two-dimension assemble function that describes joint phase-matching, while the function f (ω1 , ω2 ) = Cl2 χ0 E0 (ω0 )e−iα(∆k1 ) e−iα(∆k2 ) , depends on the parameters of three-wave interaction, the phase multipliers α(∆ki ) = N2l [(∆ki −G)+(M −1)(∆ki −F )] in the formula (5) and C is the normalization factor of three-photon amplitude. Three-photon down-conversion is controlled by energy conservation between the pump and daughter ′ photons ω0 = ω1 + ω1 + ω1” . Analyzing the graphics of YM,N (x) (see Fig. 3) in application to cascaded scheme of down-conversion we could arrange two twin peaks of the phase-matching function with the wave-vector mismatches of cascading processes. We demonstrate it using the experimental dates for the cascaded down-conversion [17]. For the typical value of pump wave length λL = 0.53µm and LiTaO3 crystal mismatch parameters from experimental results are ∆k1 = 0.32µm−1 and ∆k2 = 0.87µm−1. We check that the simultaneous phase-matching of two processes is really realized on the formula (6) for the parameters: l = 10.25µm, N = 22, M = 9. In this case, the ∆k1 match with the second peak of the first twin-peaks on the positive branch of the axes and the ∆k2 matches with the first peak of the second twin-peaks, which are situated next to the first twin-peaks and separated from them by the period. We got perfect correspondence of theoretical and experimental results. The dependence of the spectral function h(x1 , x2 ) on the parameters x1 and x2 is shown in Figs. 5,6. As we see, the joint spectral function displays the various maxima in x1 , x2 place that indicate the range of the results of the effective three-photon splitting and perfectly confirm the results exhibited in Fig. 2. Thus, the above results show that the efficient generation of three-photon subharmonic mode is possible in this scheme. The parametric gain of the three-photon down-conversion in the spectral range of the maxima of the function h(x1 , x2 ) is the result of the most simultaneous phase-matching of two cascading second-order processes. In the end of the section we shortly discuss QPM for generation of four-photon states in cascaded parametric oscillator. This device consists of three intracavity modes. The pump mode driven by an external coherent driving field at the frequency ̟0 is converted into the pair of modes ̟2 , where ̟0 = ̟2 + ̟2 = 5 0.4 0.3 0.2 6000 13,32 0.4 0.1 4000 1.50 1.55 1.60 0.2 h(x ,x2) 2000 1 0 -4 -2000 2 -2 4 x -0.2 1.8 1.6 1.4 -4000 1.2 1.8 1.0 1.2 x 1.4 2 1.6 1.4 1.6 1.2 x 1 1.8 1.0 FIG. 5: The detailed plot of the function h(x1 , x2 )in the range of double phase-matching peaks: 1 < x1 < 2 and 1 < x2 < 2, and the parameters N = 22, M = 8. There are four peaks: two positive , which are correspond to x1 = 1.5, x2 = 1.5, x1 = 1.64, x2 = 1.64, and two negative at x1 = 1.5, x2 = 1.64 and x1 = 1.64, x2 = 1.5. 2000 FIG. 7: Plot of the function YM,N (x) for the parameters for simultaneous QPM of four-photon down conversion. The number of domains is N = 32 and that of the blocks is M = 13. The insert is detailed the structure of twin-peaks. reversed crystal mismatch vectors are ∆k1 = 1, 56µm−1 ∆k1 = −1, 312µm−1, these parameters are taken from the experimental results for fourth-harmonic generation [18]. We found the parameters of the phase-reversed structure for simultaneous realization of the four-photon down-conversion. QPM of mentioned process is realized and perfectly matched with the experimental results for parameters l = 2, 2µm, M = 13 and N = 32 (see, Fig. 7). 1500 1000 1 h(x ,x2) 500 IV. 0 CONCLUSION -500 1.8 1.6 -1000 1.4 1.2 1.8 -1500 1.0 2 1.4 x 1.6 4.4 4.6 1.2 x 1 4.8 5.0 1.0 FIG. 6: Plot of the function h(x1 , x2 ) in the ranges 4.2 < x1 < 5 and 1 < x2 < 2, and the parameters N = 22, M = 9. The heights of the peaks are three times lower than for the peaks displayed on Fig. 5 in an agreement with the results presented on Fig. 2. ω0 /2 + ω0 /2. Then, each of the mode ̟2 is transformed into second pair of modes ̟1 , where ̟2 = ̟1 + ̟1 = ̟0 /4 + ̟0 /4. These processes are characterized by the wave-vector mismatches: ∆k1 = k(̟0 ) − 2k(̟2 ) and ∆k2 = k(̟2 ) − 2k(̟1 ), respectively. To realize QPM, we use the typical value of four-photon down-conversion pump wave length λp = 0, 39µm. In LiTaO3 phase- In conclusion, we have analyzed phase-reversed QPM structures in superlattice as the ensemble of domains and blocks of second-order nonlinear layers. In the result, the effective nonlinear coefficient G(∆k) of three-wave interaction has been obtained as the product of the standard phase-matching spectral function for a single segment and the assemble function. Generally used phenomenological method for description of multilayered structures required huge number of domains and blocks to provide the periodicity of the function. Our investigations shows that the detailed method we have used for description of the systems qualitatively matches with phenomenological results for the big number of domains N and blocks M , moreover, it is applicable for the finite number of layers. The results shows that we can QPM various multiphoton processes managing number of domains and blocks. We have demonstrated that double phase-matched interaction on the base of phase-reversed QPM structures in superlattice becomes possible in a wide region of the optical wavelengths, particularly, for production of muliphoton states. 6 Acknowledgments This work was partially supported by ISTC, grants A1517 and CRDF/NFSAT/SCS No. ECSP-09-53 A-03. [1] S.M. Saltiel, A.A. Sukhorukov, Y.S. Kivshar in: E. Wolf, Progress in Optics, Vol. 47, Elsevier B.V. (2004), pp. 173. [2] D.S. Hum, and M.M. Fejer, C. R. Physique 8 (2007) 180198. [3] P. Kok, W. J. Munro, K. Nemoto, T.C. Ralph, J.P. Dowling, and G.J. Milburn, Rev. Mod. Phys. 79 (2007) 135175. [4] J.L. O’Brien, Science 318 (2007) 1567-1570. [5] P.M. Leung, W.J. Munro, K. Nemoto, and T.C. Ralph, Phy. Rev. A 79, 042307 (2009). [6] P.M. Leung, T.C. Ralph, W.J. Munro, and K. Nemoto, arXiv/quant-phys. 0810.2828L (2008). [7] M. H. Chou, K. R. Parameswaran, and M. M. Fejer, Opt. Lett. 24, 16 (1999) 1157-1159. [8] Z.W Liu, S.N. Zhu, Y.Y. Zhu, Y.Q. Qin, J.L. He, C. Zhang, H.T. Wang, N.B. Ming, X.Y. Liang, and Z.Y. Xu, Jpn. J. Appl. Phys. 40 (2001) 6841-6844. [9] Z.W Liu, Y. Du, J.Liao, S.N. Zhu, Y.Y. Zhu, Y.Q. Qin, H.T. Wang, J.L. He, C. Zhang, and N.B. Ming, J. Opt. Soc. Am. B 19 (2002) 1676-1684. [10] D.N. Klyshko, JETP 77, 222 (1993). [11] A.B. U’Ren, C. Silberhorn, K. Banaszek, I.A. Walmsley, R.K. Erdmann, W.P. Grice, and M.G. Raymer, Quant.Opt. 15 (2005) 146-161. [12] K.J. Resch , Ph. Walther , A. Zeilinger, Phys. Rev. Lett. 94(7), 070402 (2005). [13] J.M. Wen, P. Xu, M. H. Rubin, and Y.H. Shih, Phys. Rev. A 76, 023828 (2007). [14] H. Hübel, D.R. Hamel, A. Fedrizzi, S. Ramelow, K.S. Resch, and T. Jennewein, Nature Photonics Lett. 466 (2010) 601-603. [15] D.A. Antonosyan, T.V. Gevorgyan, and G.Yu. Kryuchkyan, Phys. Rev. A 83, 043807 (2011). [16] M. Atatüre, A.V. Sergienko, B.E. A. Saleh, and M.C. Teich, Phys. Rev. Lett. 86 (2001) 4013-4016. [17] D. Kolker,A.K. Dmitriyev, P.V. Gorelik, F.N.C. Wong, and J.J. Zondy, Laser Phys. 18(6) (2008) 794799. [18] A.A. Sukhorukov, T.J. Alexander, Yu.S. Kivshar, S.M. Saltiel, Physics Letters A 281, (2001) 34-38.